advertisement

Wrinkling of Orthotropic Viscoelastic Membranes X. Deng∗ and S. Pellegrino† California Institute of Technology, Pasadena, California 91125 This paper presents a simpliﬁed simulation technique for orthotropic viscoelastic ﬁlms. Wrinkling is detected by a combined stress-strain criterion and an iterative scheme searches for the wrinkle angle using a pseudo-elastic material stiﬀness matrix based on a nonlinear viscoelastic constitutive model. This simpliﬁed model has been implemented in ABAQUS/Explicit and is able to compute the behavior of a membrane structure by superposition of a small number of response increments. The model has been tested against a published solution for a time-independent isotropic membrane under simple shear and also against experimental results on StratoFilm 420 under simple shear. I. Introduction Wrinkling of thin membranes has attracted much interest and yet little is known about wrinkles in anisotropic viscoelastic membranes. Our interest in this topic is motivated by current research in superpressure balloons, and particularly their behavior during inﬂation when the balloon envelope is heavily wrinkled. In recent papers1, 2 we have presented numerical simulations of some particular balloons that remain clefted when they are fully inﬂated and pressurized. These results were in agrement with experimental tests that had been conducted by the NASA Balloon Program, but the shape of the clefts in our simulations did not agree with the experimental observations. It was conjectured that these discrepancies may have resulted from the elastic and isotropic model for the balloon ﬁlm that had been used and so it was decided to implement a more detailed material model that allowed for both anisotropy and visco-elasticity. However, when wrinkling had been combined with these eﬀects we were unable to ﬁnd any published test cases that could be used to conﬁrm the validity of our simulations and so we decided to carry out our own set of experiments as well. We intend to study how these eﬀects aﬀect the shape of clefts in superpressure balloons, these results will be presented in future publications. Here we present the outcome of our studies on wrinkling in moderately anisotropic, viscoelastic thin ﬁlms. The paper begins with a literature review focused on a particular nonlinear viscoelastic material model for balloon ﬁlm and an approach to the numerical simulation of wrinkling in anisotropic ﬁlms. With this key background, in Section III we present a computational scheme that models the visco-elasticity of the ﬁlm with an incremental, pseudo-elastic representation that is modiﬁed to allow for the formation of wrinkles, when a combined stress-strain wrinkling criterion is satisﬁed. This scheme is then implemented, in Section IV, as a VUMAT subroutine in the ﬁnite element software Abaqus/Explicit. Section V considers the special case of isotropic and elastic membranes, for which there is an extensive literature, and compares the results from our simulations to some published results. Section VI presents a set of experiments that have been carried out on balloon ﬁlm in a simple shear apparatus; the experimental setup and procedure are described and the results of shear tests are presented. In Section VII these experimental results are compared with the simulations. Section VIII concludes the paper. II. Background This section provides a compact review of viscoelasticity and wrinkling theories for orthotropic thin polymeric ﬁlms. ∗ Graduate Student, Graduate Aerospace Laboratories, 1200 East California Boulevard. and Kent Kresa Professor of Aeronautics and Professor of Civil Engineering, Graduate Aerospace Laboratories, 1200 E. California Blvd. MC 301-46. AIAA Fellow. [email protected] † Joyce 1 of 23 American Institute of Aeronautics and Astronautics A. Review of Viscoelasticity Theory In the classical theory of linear viscoelasticity3, 4 the creep compliance D and relaxation modulus E can be obtained from spring and dashpot models. A spring in series with a dashpot is known as the Maxwell model; a spring in parallel with a dashpot is known as the Kelvin-Voigt model. Both models have serious shortcomings. A more realistic model is the Standard Linear Solid model which is either represented by a Maxwell element with an additional spring in parallel or a Kelvin-Voigt element with an additional spring in series. A more realistic representation of actual viscoelastic behavior is obtained by considering n Kelvin-Voigt elements with one spring in series, which leads to a compliance function expressed as a sum of exponential terms called Prony series n D(t) = D0 + ΔDi (1 − e−t/τi ) (1) i=1 Viscoelastic materials are temperature as well as time dependent but both eﬀects can be combined through the time-temperature superposition principle by considering only the reference temperature T0 and the reduced time t dτ (2) ψ(t) ≡ a (T ) T 0 where aT (T ) is the temperature shift factor, deﬁned to be 1 at the reference temperature (aT (T0 ) = 1). The compliance master curve, which deﬁnes the time-dependent compliance at the reference temperature, can be obtained from a series of uniaxial creep tests. It can be expressed as a combination of an instantaneous part D0 and a transient part ΔD(ψ): D(ψ) = D0 + ΔD(ψ) (3) Here D0 represents the instantaneous compliance at the reduced time ψ = 0 and the transient part ΔD(ψ) can be represented by the Prony series: ΔD(ψ) = n Di (1 − e−ψ/τi ) (4) i=1 The linear viscoelastic strain at time t, (t), is calculated by the convolution integral (also called Boltzman Superposition integral) t dσ(τ ) dτ ≡ D(ψ)σ(t) (5) ΔD(ψ t − ψ τ ) (t) = D0 σ(t) + dτ + 0 Experimental studies have shown that this linear model is acceptable at small strains, whereas nonlinear eﬀects tend to become signiﬁcant at strains generally larger than 0.5%. At larger strains a nonlinear viscoelastic model has to be adopted, where the creep compliance is a function of stress, as well as of time and temperature. Following Schapery5, 6 this behavior can be captured by introducing an experimentally derived stress-related shift aσ in the reduced time expression, which kicks in at stresses higher than a limiting value σ0 . Hence Equation 2 for the reduced time is rewritten as t dτ (6) ψ(t) ≡ a (T )a T σ (σ, T ) 0 Schapery5 has adopted a single-integral representation for the strain at time t based on three nonlinear parameters g0 , g1 and g2 : t dg2 σ(τ ) dτ ≡ D(ψ) ∗ σ(t) (7) ΔD(ψ t − ψ τ ) (t) = g0 D0 σ(t) + g1 dτ 0+ where the nonlinear parameters are all equal to 1 in the linear viscoelasticity range. The above uniaxial model has been extended5 to plane stress loading of a polymeric ﬁlm by making the assumption that the transient compliance in any direction can be expressed in terms of a constant matrix Sij multiplied by the compliance in a direction of orthotropy of the material, assumed to be known ΔDij = Sij ΔD11 2 of 23 American Institute of Aeronautics and Astronautics (8) where S11 = 1 by deﬁnition. The uniaxial stress σ used to calculate all stress-dependent non-linearities in the previous model is then replaced with an eﬀective stress. This is deﬁned as 2 2 2 (9) σeﬀ = σ 11 + 2A12 σ 11 σ 22 + A22 σ 22 + A66 τ 12 where σ 11 is the normal stress in the one of the directions of material orthotropy, and it is assumed that the uniaxial model has been developed in this particular direction, σ 22 is the normal stress in the other direction of orthotropy, and τ 12 is the shear stress. The notation denotes components in the directions of orthotropy. B. Wrinkling of Orthotropic Films There is an extensive literature on wrinkling of thin elastic ﬁlms; the interested reader is referred, for example, to Wong and Pellegrino7–9 for a general review. Here we shall focus speciﬁcally on wrinkling in orthotropic ﬁlms, for which the literature is rather scarce. Kang and Im10 proposed an iterative scheme for the ﬁnite element analysis of wrinkling in orthotropic membrane structures, which was later adopted by Gerngross and Pellegrino.11–13 Alternative approaches have been proposed by Epstein and Forcinito14 and Raible et al.15 The general idea in Kang and Im’s paper is that a wrinkled region in a thin ﬁlm is in a state of uniaxial tension and the orientation and magnitude of this tension can be obtained from an invariant relation between strain components. The actual wrinkled shape of the ﬁlm is not of interest, instead a ﬁctitious non-wrinkled surface is used to describe the average deformation of the ﬁlm. Consider an undeformed material element ABCD, Figure 1(a). Let ( x, y) denote a Cartesian coordinate system in the undeformed conﬁguration, where x , y are aligned with the directions of orthotropy of the material. Let (x, y) denote a rotated Cartesian coordinate system for the same material point but such that x is the direction of the uniaxial stress in the wrinkled material. The rigid body rotation angle, α, from x y to xy is called the wrinkling angle. It is noteworthy that for isotropic materials the wrinkling angle is the same as the principal stress or strain angle but this is generally not the case for anisotropic materials. After this rigid body rotation, the material element, which is now considered in a rotated Cartesian coordinate system, is transformed from the undeformed conﬁguration ABCD to the ﬁnal, wrinkled conﬁg uration A B C D in two steps, Figure 1(b). The ﬁrst step is a pure deformation from the undeformed conﬁguration ABCD to the deformed conﬁguration A B C D , due to the application of the correct uniaxial stress σx . No wrinkling occurs during this deformation, because there are no constraints on the deformation kinematics. This deformation consists of a normal strain ux , a transverse contraction uy (due to the Poisson’s u ratio of the membrane), and an additional shear strain γxy (only in the case of anisotropic materials). This strain state is called the state of natural uniaxial tension and the superscript u has been used to denote the corresponding strains. The second step involves pure wrinkling from A B C D to A B C D . During this step, the stress in the material does not change and hence its strain state also does not change, but the material element “shrinks” due to the formation of a series of wrinkles. At this point, though, the actual material element (which is no longer planar) is replaced by a ﬁctitious wrinkled surface with the same outer proﬁle. Let e1 and e2 be unit vectors denoting respectively the x and y direction. The material point X = X1 e1 + X2 e2 in the reference conﬁguration ABCD corresponds to point x = x1 e1 + x2 e2 in the state of natural uniaxial tension (i.e., in conﬁguration A B C D ) and to point xu = xu1 e1 + xu2 e2 in the ﬁnal deformed conﬁguration A B C D . The mapping from ABCD to A B C D is written as xu1 = au X1 + cu X2 and xu2 = bu X2 , and the mapping from ABCD to A B C D is written as x1 = aX1 + cX2 and x2 = bX2 . During the wrinkling process, the points A , B , C , D move vertically to A , B , C , D , therefore there is no deformation of e2 , but there is still contraction of e1 , i.e. a = au , c = cu and b ≤ bu (10) The Green strain tensors for the ﬁctitious wrinkled state and the state of natural uniaxial tension are 1 2 1 1 (a − 1)e1 ⊗ e1 + ac(e1 ⊗ e2 + e2 ⊗ e1 ) + (b2 + c2 − 1)e2 ⊗ e2 2 2 2 = x e1 ⊗ e1 + xy e1 ⊗ e2 + yx e2 ⊗ e1 + y e2 ⊗ e2 = 3 of 23 American Institute of Aeronautics and Astronautics (11) 1 u 2 1 1 [(a ) − 1]e1 ⊗ e1 + (au )(cu )(e1 ⊗ e2 + e2 ⊗ e1 ) + [(bu )2 + (cu )2 − 1]e2 ⊗ e2 2 2 2 = ux e1 ⊗ e1 + uxy e1 ⊗ e2 + uyx e2 ⊗ e1 + uy e2 ⊗ e2 u = (12) Comparing the above three equations, we conclude that in the wrinkled state the strain components x u and γxy remain unchanged, i.e. x = ux and γxy = γxy , but the transverse strain y is diﬀerent due to the over-contraction of the material in the direction perpendicular to the stress direction, i.e. uy ≥ y . A y Natural uniaxial tension membrane B B’ y (e2) B’’ A B A’ A’’ y σx x α x (e1) x C’’ D’’ D’ D C D C Wrinkling orientation C’ Fictitious surface Undeformed membrane (b) Wrinkling process of deformed configurations (a) Rigid body rotaion of Cartesian coordinate system Figure 1. States of a wrinkled element Assuming that the Green strain in the membrane is small, it is approximately equal to the standard Cauchy strain and so the stress-strain relationship has the standard linear form ⎤ ⎡ ⎫ ⎫ ⎧ ⎧ C 0 C 11 12 ⎪ ⎪ x ⎬ ⎢ ⎬ ⎥ ⎪ ⎨ σ ⎨ x ⎪ ⎥ ⎢ =⎢ C (13) · ⎥ C σ y 0 21 22 y ⎪ ⎪ ⎪ ⎦ ⎪ ⎭ ⎣ ⎭ ⎩ ⎩ τ γxy xy 0 0 C 66 }. Note that the shear-extension coupling terms which can be written in the compact form { σ } = [C]{ in this material stiﬀness matrix [C] are zero because the relationship has been set up in the directions of orthotropy of the material. This stress-strain relationship can be transformed to the x, y coordinate system by rotating through the angle α ⎡ ⎤ ⎫ ⎫ ⎧ ⎧ C11 C12 C16 ⎪ ⎪ ⎥ ⎪ ⎬ ⎨ x ⎪ ⎨ σx ⎬ ⎢ ⎢ ⎥ = ⎢ C21 C22 C26 ⎥ · (14) σy y ⎪ ⎪ ⎪ ⎦ ⎪ ⎭ ⎣ ⎭ ⎩ ⎩ τxy γxy C61 C62 C66 or {σ} = [C]{}. Here {} can be obtained from { } by the transformation [C] = [T ][C][R][T ]−1 [R]−1 where [R] = diag{1, 1, 2} and ⎡ ⎢ ⎢ [T ] = ⎢ ⎣ cos2 (α) sin2 (α) sin2 (α) cos2 (α) − sin(α) cos(α) sin(α) cos(α) 2 sin(α) cos(α) (15) ⎤ ⎥ ⎥ −2 sin(α) cos(α) ⎥ · ⎦ 2 2 cos (α) − sin (α) 4 of 23 American Institute of Aeronautics and Astronautics (16) The wrinkling angle α has to be such that the normal stress in the direction perpendicular to the wrinkles u is zero and the shear stress is also zero, that is σyu = τxy = 0. If this condition is satisﬁed, then the transverse u can be obtained from strain uy and the shear strain γxy uy = ux C21 C66 − C26 C61 C26 C62 − C22 C66 (17) C22 C61 − C21 C62 C26 C62 − C22 C66 (18) u = ux γxy Kang and Im10 proposed an iterative approach to search for the wrinkling angle. The procedure to ﬁnd u α is a follows. First, one determines a value of α that satisﬁes the relationship γxy = γxy , with ux = x . u u Here, y and γxy are calculated from Equations 17 and 18. Finding α is equivalent to solving the equation u (α) − γxy (α) = 0 f (α) = γxy (19) which may have multiple solutions between 0 and 180 degrees. To ﬁnd all of the solutions, we ﬁrst divide the domain into ten uniform intervals and look for a change of sign between two boundary points in any interval. If a change of sign is found, then there is at least one solution inside this particular interval. Then we iteratively calculate the intersection between a straight line connecting two boundary points and the x-axis until the error is less than a prescribed tolerance. Once we have found a value of α that satisﬁes this equation, we check that uy ≥ y and if this inequality is satisﬁed, then α deﬁnes the wrinkling orientation. If no change of sign is found, the domain is divided into 50 intervals and the calculation is repeated. III. Eﬀective Material Stiﬀness Matrix A particular balloon ﬁlm, StratoFilm 420, will be considered in this study. This ﬁlm has been extensively characterized by Rand.16, 17 In the ﬁrst part of this section we review the nonlinear viscoelastic properties of Stratoﬁlm 420 and then develop an approximate pseudo-elastic constitutive model for a chosen temperature, time interval and stress level. In the second part of the section we modify the pseudo-elastic coeﬃcients to consider the eﬀects of wrinkling. A. Pseudo-elastic model for StratoFilm 420 StratoFilm 420 is a 38 micron thick ﬁlm made of Linear Low Density Polyethylene.18 Rand16, 17 has developed a nonlinear viscoelastic constitutive model for this ﬁlm. The transient compliance ΔD(T0 , ψ) in the machine direction of the ﬁlm was given at a reference temperature T0 =293.16 K and the instantaneous compliance D0 = 3.0 × 10−10 (Pa−1 ) was chosen to ensure that the transient compliance Di would all be positive. The coeﬃcients of a 15 term Prony series are listed in Table 1. The temperature shift factor aT was evaluated over the range 163 K to 323 K and then ﬁtted at the reference temperature T0 = 293.16K in the logarithmic form ⎧ ⎨ (T − 293.16)[7.33 × 10−4 (T − 273.16) − 0.179133] T > 233.16 log aT = (20) ⎩ 3.1068 − 0.2350275(T − 273.16) T < 233.16 The stress shift was represented by aσ log aσ = −0.126(σeﬀ − σ0 ) (21) where σ0 is threshold at which linear behavior ends and nonlinear behavior begins σ0 = 69.527 − 0.430944T + 6.7962 × 10−4 T 2 (22) Two of the non-linear coeﬃcients, g0 and g1 were set equal to 1. The parameter g2 was described by g2 = 1 + 0.1875(σeﬀ − σ0 ) 5 of 23 American Institute of Aeronautics and Astronautics (23) Table 1. Prony series for StratoFilm SF420 Di (MPa−1 ) 1.8764×10−4 2.9249×10−5 5.8224×10−5 8.7542×10−5 1.1561×10−4 1.4159×10−4 1.6989×10−4 2.0924×10−4 2.7274×10−4 3.7796×10−4 5.4670×10−4 8.0581×10−4 1.1844×10−3 1.7204×10−3 2.6285×10−3 i 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 τi (s) 1.6548×10−16 4.8697×10−15 1.4330×10−13 4.2170×10−12 1.2409×10−10 3.6517×10−9 1.0746×10−7 3.1623×10−6 9.3057×10−5 2.7384×10−3 8.0582×10−2 2.3714 69.783 2053.5 60430 The coeﬃcients for the biaxial model were, in addition to S11 = 1, S22 = 1.122 + 6.5895 × 10−4 T − 6.609 × 10−6 T 2 (24) and S12 = S21 = −0.58, S66 = 4.45. The coeﬃcients for the eﬀective stress, Aij , were expressed as A22 = 1.44, A12 = −0.4 and A66 = 0.8 (25) A ﬁnite-element implementation of the above constitutive model for the analysis of a single balloon lobe has been developed by Gerngross and Pellegrino11–13 model. Here we present an alternative approach that, although less accurate, is more suitable for large scale simulations of balloon structures. For a given time t, the integral representation for the strain (t) in Equation 7 can be approximated by t where each term is evaluated replacing the convolution integral with a series of m equal substeps Δt = m at the discrete time ti = iΔt (t) ≈ g0 D0 σ(t) + g1 m ΔD(ψ t − ψ ti−1 )Δ[g2 (σ ti )σ(ti )] i=1 = g0 D0 σ(t) + g1 m ΔD(ψ t − ψ ti−1 )[g2 (σ ti )σ(ti ) − g2 (σ ti−1 )σ(ti−1 )] (26) i=1 Substituting g0 = g1 = 1 and assuming that g2 changes slowly over Δt, i.e. g2 (σ ti ) ≈ g2 (σ ti−1 ), then the above equation becomes (t) ≈ D0 = m m i=1 Δσ(ti ) + m g2 (σ ti )ΔD(ψ t − ψ ti−1 )Δσ(ti ) i=1 [D0 + g2 (σ ti )ΔD(ψ t − ψ ti−1 )]Δσ(ti ) (27) i=1 Hence, we can deﬁne a pseudo-elastic compliance, Dp,i (the superscript p corresponds to ”pseudo-elastic”) between iΔt and t, and considering the corresponding reduced times 6 of 23 American Institute of Aeronautics and Astronautics Dp,i = D0 + g2 ΔD(ψ t − ψ ti−1 ) (28) The corresponding strain can then be expressed as (t) = m Dp,i Δσ(ti ) = i=1 m Δ(ti ) (29) i=1 This uniaxial expression can be generalized to plane stress by deﬁning the pseudo-elastic compliance in p,i , from Equation 28 the machine direction, D 11 p,i = D0 + g2 ΔD(ψ t − ψ ti−1 ) D 11 (30) and the remaining coeﬃcients of the pseudo-elastic compliance matrix are then p,i = S22 D p,i , D p,i , D p,i p,i = D p,i = S12 D p,i = S66 D D 22 11 12 21 11 66 11 (31) It follows from Equation 29 that the strain at time t can be obtained as a sum of strain increments, which are calculated from the stress increments multiplied by the corresponding total pseudo-elastic compliances. For each increment, the pseudo-elastic compliance is constant. For example, if we consider the conditions of constant temperature T = 293 K, constant stress σ x = 4.5 MPa, σ y = 5.0 MPa and τ = 0 MPa, the shift of the compliance master curve in the machine direction xy is shown in Figure 2. At time t = 1000 s, the pseudo-elastic moduli can be obtained from the compliance at p = 121.68 MPa. p = 90.98 MPa and E the point marked with a dot in Figure 2. They are respectively E 11 22 1.8 x 10 −8 Compliance D [1/Pa] real time reduced time 1.2 0.6 0 −15 −10 −5 log t [s] 0 3 5 Figure 2. Master curves of compliance in machine direction. The pseudo-elastic stiﬀness matrix in the directions of orthotropy of the ﬁlm can be obtained by inversion p,i of D ⎤ ⎡ p,i p,i E 0 E 11 12 ⎥ ⎢ ⎥ p,i = ⎢ p,i E p,i E (32) ⎢ E 0 ⎥ 21 22 ⎦ ⎣ p,i 0 0 E 66 where p,i E 11 = 1 p,i D11 1 2 /S S11 − S12 22 7 of 23 American Institute of Aeronautics and Astronautics B. p,i E 12 = p,i E 22 = p,i E 66 = 1 p,i E21 = 1 p,i S D11 12 − S11 S22 /S12 1 1 2 p,i S D11 22 − S12 /S11 1 1 p,i S D11 66 Correction for Wrinkling Kang and Im10 compared three types of wrinkling criteria, the principal stress criterion, the principal strain criterion and the mixed criterion. They concluded that the mixed criterion works better for anisotropic wrinkling as it avoids numerical divergence caused by making wrong judgements about the membrane state, which happened with the principal stress based criterion. The eﬀective elasticity matrix depends on the state of a membrane element: • Minor principal stress σ2 > 0: the membrane is taut, hence Equation 32 is valid. • Minor principal stress σ2 ≤ 0 and major principal strain ε1 > 0: the membrane is wrinkled. Hence we must solve for the wrinkling angle α. First we transform the pseudo-elastic stiﬀness in Equation 32 to the rotated coordinate system x, y (the transformation is analogous to Equation 14). In this system, the normal strain x and the shear strain γxy are equal to the strains in the state of natural uniaxial tension whereas y is not. The transverse stress σy has to be zero in a coordinate system aligned with the wrinkles, hence p,i p,i p,i x + E22 y + E23 γxy = 0 σy = E21 (33) From the above equation, y can be expressed in terms of x and γxy . y = − p,i E21 p,i x − E22 p,i E26 p,i E22 γxy (34) Hence we eliminate y by substituting this expression into Equation 14, ticity matrix13 for the wrinkled element ⎡ p,i E p,i E p,i E p,i E p,i p,i − 12E p,i26 E11 − 12E p,i21 0 E13 22 22 ⎢ ⎢ p,i Ew = ⎢ 0 0 0 ⎢ ⎣ E p,i E p,i E p,i E p,i p,i p,i − 62E p,i21 0 E66 − 26E p,i62 E61 22 and obtain the eﬀective elas⎤ ⎥ ⎥ ⎥ ⎥ ⎦ (35) 22 An alternative method is using directly the strains in the state of natural uniaxial tension {u } from Equations 17 and 18. Hence the corrected stress in the wrinkled state {σ} has to be a uniaxial tension, rewritten as {σ} = {σ u } = E p,i {u }. Since the element is under uniaxial tension, only the x component σx is nonzero. Finally {σ} is transformed back to { σ } in the direction of orthotropy. • Major principal strain ε1 ≤ 0 and minor principal stress σ2 < 0: the membrane is slack and hence Esp,i = [0] In conclusion, to calculate the correct stress, the following steps are carried out: Step 1. Check the state of the membrane element by means of the mixed criterion; Step 2. If the element is wrinkled, ﬁnd the wrinkling angle α from Kang and Im’s scheme, described in Section 2; Step 3. Compute the corrected Cauchy stress using the eﬀective elasticity matrix. The stress and strain components used for the above wrinkling tests should ideally be the best current estimates of the values at time t. However our current approach is to run each step i as a separate simulation in ABAQUS/Explicit and hence the only estimates that are available in each run are only the estimates based on the current increment. 8 of 23 American Institute of Aeronautics and Astronautics IV. Finite Element Implementation In Section III we have presented an approach to obtain approximate estimates of the stresses in a viscoelastic ﬁlm at time t. The loading sequence is divided into m steps, where m is determined by the required precision, and m m p,i Δ(ti ) E Δσ(ti ) = (36) σ(t) = i=1 i=1 For example, the strain increments due to a three step loading sequence are shown on the left of Figure 3(a), hence (37) = Δ1 + Δ2 + Δ3 The stress at the end time, t3 , due to the strain increments Δi is computed with ABAQUS/Explicit in p,i . The results are shown in Figure 3(b-d) and are superposed three separate analyses with compliances E in Figure 3(a). From the plots on the right in Figure 3, the stress at time t3 is given by σ(t3 ) = = Δσ1 + Δσ2 + Δσ2 E p,1 Δ1 + E p,2 Δ2 + E p,3 Δ3 (38) Note that an approximation in this approach is to assume that the wrinkling directions in each step will not change signiﬁcantly between the various steps,. Also, the coeﬃcient g2 is stress-dependent and so is not correctly estimated for the full stress level. In other words, the proposed linear superposition is suitable for weakly nonlinear materials with only small wrinkle angle changes. A user-deﬁned material ABAQUS/Explicit subroutine (VUMAT) has been written to model wrinkling in an orthotropic viscoelastic ﬁlm, it is schematically described in Figure 4. V. Veriﬁcation for Isotropic Elastic membranes We have tested our VUMAT implementation of wrinkling in ABAQUS/Explicit by means of a comparison with the analytical solution for a linear-elastic, time-independent rectangular membrane under simple shear. The longer edges of the membrane are attached to rigid edges that are sheared uniformly while the shorter edges are unconstrained. This problem was investigated by Wong and Pellegrino.9 A. Construction of FE Model This test case involves a rectangular membrane under simple shear. The properties of the ﬁlm used in the model and the geometrical dimensions of the rectangular membrane are summarized in Table 2. Table 2. Summary of membrane properties Length, L (mm) Height, H (mm) Thickness, t (mm) Young’s Modulus, E (N/mm2 ) Poisson’s ratio, ν Density, ρ (kg/mm3 ) 380 128 0.025 3530 0.33 1.46×10−6 The membrane was modeled with 3-node, fully integrated triangular membrane elements (M3D3). All translations of the bottom edge nodes were fully constrained, whereas the top edge nodes were left free. As shown in Figure 5, the shear load was applied in terms of a horizontal shear displacement of the top edge. The loading process consisted of two analysis steps: during the ﬁrst step, lasting 2.5 seconds, the upper edge nodes were moved by 3 mm in the x-direction while all other translations were constrained. In the second step, also lasting 2.5 seconds, all the translational degrees of freedom on the upper and lower edges were constrained, to test the stability of the simulation. 9 of 23 American Institute of Aeronautics and Astronautics Stress σ Strain ε ε3 ε2 σ(t3) ε1 t0 t1 t2 Real time t t0 t3 t1 t2 Real time t t3 Strain Stress σ ε (a) Δε1 = ε1 Δσ1 t0 t1 t2 Real time t t3 t0 t1 t2 Real time t t3 Strain ε Stress σ (b) Δε2 = ε2 − ε1 Δσ2 t0 t1 t2 Real time t t3 t0 t1 t2 Real time t Strain ε Stress σ (c) t3 Δε3 = ε3 − ε2 t0 t1 t2 Real time t Δσ3 t0 t3 t1 t2 Real time t t3 (d) Figure 3. Superposition of loading steps: (a) total strain input and stress response; (b)−(d) incremental strain functions and corresponding stress responses. 10 of 23 American Institute of Aeronautics and Astronautics In p u t fro m A B A QU S : N ew strain, old stress , real loading tim e, tem perature Compute pseudoelastic stiffness matrix slack taut M ixed w rinkling criterion w rinkled D eterm ine w rinkle angle R otate coordinate system into w rinkling direction Stiffness m atrix based on linear elastic orthotropic relation M odify stiffness m atrix as effective elasticity m atrix Set stiffness m atrix = 0 D eterm ine uniaxial stress R otate coordinate system back to m aterial direction Ou tp u t to A B A QU S : N ew stress Figure 4. Wrinkling algorithm for linear orthotropic viscoelastic material subroutine VUMAT 11 of 23 American Institute of Aeronautics and Astronautics H= 128 mm δx = 3 mm Y X L= 380 mm Figure 5. Finite element mesh for membrane in shear B. Results The stress distribution corresponding to the ﬁnal value of the horizontal displacement of the membrane is illustrated by means of contour plots and a vector plot, in Figure 6. Since the major principal stress, σ1 , is much greater than the minor principal stress, σ2 , only the major stress can be seen in the vector plot. The direction of the major principal stress, inclined at 45◦ , corresponds to the direction of the wrinkles. The dense distributions of vectors at the top-right and bottom-left corners indicate two areas of stress concentration. The membrane ﬁnite element model using the VUMAT subroutine has succeeded in eliminating all negative stress, as illustrated by the minor stress distribution being approximately non-negative everywhere. The principal stresses across the middle of the membrane are plotted in Figure 7. σ1 increases from zero at the edge to a uniform and positive value, σ1 =41.36 MPa, whereas σ2 remains approximately zero. The major principal strain is at 45◦ and given by Wong and Pellegrino8 1 = γ 2 (39) Since the shear strain is γ = δx /H, σ1 = E1 =41.37 MPa. A detailed simulation with a thin-shell model of the membrane was carried out by Wong and Pellegrino9 and the stress distribution obtained from that approach has been plotted for reference in Figure 7. The energy variation during the Explicit simulation has been shown in Figure 9. The viscous dissipation is negligible (the linear viscosity coeﬃcient was set equal to 0.005) and the kinetic energy is also small, indicating that a quasi-static simulation has been achieved. A constant strain energy level of 236.76 mJ during the second step indicates that the simulation is stable. VI. Experimental Studies of Viscoelastic Orthotropic Membranes A rectangular membrane with exactly the same dimensions as the one considered in Section V.A and subject to the same loading condition has been tested. However, now the situation is diﬀerent in the following respects: (1) the membrane is StratoFilm 420, which is an orthotropic material showing nonlinear viscoelastic eﬀects; (2) both loading and unloading are measured and hysteretic curves obtained from experiments will be compared with results of pseudo-elastic simulations; (3) after a linear ramp loading, the imposed displacement is kept constant for a certain time before unloading, to observe the viscoelastic response. A. Shear Test Rig The shear rig is shown in Figure 10, note that the moving edge block is attached to four linear bearings (LUI 5AL). A key step in the preparation for a test is setting up the ﬂat membrane surface without any visible imperfections. To do this, a mist of distilled water was sprayed on a ﬂat Perspex sheet and a piece of StratoFilm 420 with the required dimensions was put on the sheet. Then the ﬁlm was lightly pressured with a hand roller to eliminate any air bubbles. The surface tension of the water at the interface holds the ﬁlms against the plastic sheet. The upper and lower edges of one side of the ﬁlm were glued to the ﬁxed and 12 of 23 American Institute of Aeronautics and Astronautics Max. In−Plane Principal +1.438e+02 +1.318e+02 +1.198e+02 +1.079e+02 +9.588e+01 +8.389e+01 +7.191e+01 +5.992e+01 +4.794e+01 +3.595e+01 +2.397e+01 +1.198e+01 +0.000e+00 (a) Major principal stress (unit: MPa) Min. In−Plane Principal +1.028e+00 +9.427e−01 +8.570e−01 +7.713e−01 +6.856e−01 +5.999e−01 +5.142e−01 +4.285e−01 +3.428e−01 +2.571e−01 +1.714e−01 +8.570e−02 −9.482e−07 (b) Minor principal stress (unit: MPa) S, Max. In−Plane Principal S, Min. In−Plane Principal S, Out−of−Plane Principal (c) Vector plot Figure 6. Plot of principal stress distribution for isotropic, time-independent membrane 13 of 23 American Institute of Aeronautics and Astronautics Principal stress ( N/mm2 ) 40 30 Major principal stress 20 Membrane solution Shell solution 10 Minor principal stress 0 0 100 200 X (mm) 300 400 Figure 7. Variation of principal stresses across middle horizontal section of isotropic, time-independent membrane Highly stressed corner A’ A B δx=3 mm Parallelogram region 45 D Slack triangle region C’ C Wrinkling orientation Figure 8. Wrinkling pattern for isotropic, time-independent membrane under simple shear Energy (mJ) 200. 150. Strain Energy Kinetic Energy Viscous Dissipation 100. 50. 0. 0. 1.0 2.0 3.0 4.0 5.0 Time (s) Figure 9. Energy variation for isotropic, time-independent membrane 14 of 23 American Institute of Aeronautics and Astronautics moving edges of the rig, then clamping strips were glued and bolted to the other side of the ﬁlm with M4 screws. A controlled displacement of the moving edge block was imposed by means of a ﬁne threaded screw, on the left-hand side of the rig and a force sensor (Futek LCM300) coaxial with the screw was used to measure the compressive contact force, F , between the screw and the moving edge block. A Keyence LK-G157 laser placed on the right-hand side (not shown in the ﬁgure) was used to measure the displacement δx and the variation of force and displacement with time were measured with a Vishay System 7000 data logger. The scanning frequency was 128 samples per second during loading and unloading and 10 per minute when the displacement was held constant. The data samples were averaged using a window of 20 data points to reduce noise. Force sensor Holder for screw Linear bearing Moving edge Screw Membrane Stationary edge Figure 10. Shear rig B. Experimental Procedure StratoFilm 420 is orthotropic due to the non-uniform biaxial stretching during production. The directions of orthotropy are the machine direction, i.e. the direction in which the ﬁlm is rolled, and the transverse direction. All experiments were carried out with the directions of orthotropy of the ﬁlm parallel to the direction of shearing. In experiments denoted with an “M” the machine direction of the ﬁlm was parallel to the direction of shearing, whereas in experiments denoted with a “T” the transverse direction of the ﬁlm was parallel to the direction of shearing. For both sets of experiments there were two levels of displacement magnitudes, approximately 2 mm and 3 mm, but only in second set the direction of motion was also reversed, after holding the displacement constant for a time TC . The test parameters are summarized in Table 3. It should be noted that at some point during the reversed direction of motion the reaction between the screw and the moving edge becomes tensile and at this point contact between the screw tip and the moving edge was lost. Hence, from this point on the motion of the moving edge was governed by the condition that the reaction force should be zero. C. Correction for Friction The motion of the moving edge of the shear rig is resisted by friction in the linear bearings. It was assumed that the static and kinetic friction coeﬃcients are equal and given by an expression of the type f = f0 + μT (40) where T is the total tension in the ﬁlm, i.e. the total force in the direction perpendicular to the moving edge. f was measured on the shear rig without the ﬁlm, by applying a known value of T and measuring the 15 of 23 American Institute of Aeronautics and Astronautics Table 3. Test parameters Test No. Direction of ﬁlm Displacement δx (mm) Temperature T (K) Loading type Linear ramp a M 2.31 294.55 Loading only b M 3.36 294.65 Loading only c T 2.39 294.65 Loading & unloading d T 3.34 294.65 Loading & unloading 5.85 10.775 10.18 16.79 15145.70 13582.83 22115.49 21962.0 N.A. N.A. 3.484 5.578 duration tL (s) Constant displacement duration tC (s) Linear ramp duration tU (s) corresponding force needed to continuously move the sliding edge block. The range of values of T that was considered was based on an ABAQUS simulation of the value corresponding to a ﬁlm subject to a shear displacement δx = 3 mm. Hence three levels of tension T were applied: 0 N, 11.121 N and 22.241 N. Since the friction force f has much smaller values than the horizontal force, a dynamic force sensor with higher precision, PCB Piezotronics Model 208C01, was used to measure the friction force. Two sets of test results have been plotted in Figure 11. The linear ﬁt, in Newtons, is given by f = +1.2976 + 0.00421 T (41) For simplicity the constant value f = 1.298 N was assumed, as it turned out that T is less than 22.241 N in all tests. In conclusion, the shear force acting on the ﬁlm, S, can be obtained by correcting the total applied force F , measured by the force sensor during the test, see Figure 12 for details: S = F − f if δ˙x > 0 S = F + f if δ˙x < 0 (42) (43) 1.6 Friction (N 1.2 0.8 Test No. 1 Test No. 2 Linear fit 0.4 0 0 5 10 15 20 Traction (N) Figure 11. Fitting of friction force3 16 of 23 American Institute of Aeronautics and Astronautics 25 T f δ F S T (a) T f δ F S T (b) Figure 12. Free bodies of sliding edge block to derive correction of shear force D. Results of Shear Tests The wrinkling pattern observed on a ﬁlm subject to a 3 mm shear displacement is shown in Figure 13. The wrinkles are almost evenly distributed in the central parallelogram region. The top left and bottom right corner regions are slack and so there are no wrinkles in these regions. Figure 13. Wrinkling pattern for 38 micron thick Stratoﬁlm 420 subject to 3 mm shear displacement A correction to the measured total force has been applied, using Equations 42 and 43 with a constant friction value, have been applied to correct the shear force, respectively for the cases of loading and unloading. The results have been plotted in Figures 14 and 15. A comparison between the shear force time variation between the four tests is shown in Figure 14. The increase in shear force is approximately linear during the loading ramp. Then it gradually decreases when the displacement remains constant and tends to a constant value. The relationship between the shear force and displacement for the four tests is shown in Figure 15. The curves for total shear displacements of 2 mm and 3 mm generally follow the same shape and kinks appear at the point of initial unloading due to the shear force correction when the friction suddenly changes direction. Clearly the simpliﬁed friction correction model that bas been used does not do a good job at the point of transition. Since the diﬀerences in corresponding displacements are minor, the temperature did not change and the loading can be assumed quasi-static, it is interesting to compare the maximum shear forces in the four tests, 17 of 23 American Institute of Aeronautics and Astronautics 10 2 10 2 Shear disp 2mm Shear disp 3mm 10 1 10 0 10 Shear force (N) Shear force (N Shear disp 2mm Shear disp 3mm −1 10 0 10 1 2 10 Time (s) (a) 10 3 10 4 10 10 1 10 0 −1 10 5 0 10 1 10 2 10 Time (s) 3 10 4 5 10 10 (b) Figure 14. Measured time dependence of shear force, after correction for friction eﬀects: (a) “M” machine direction parallel to direction of shearing; (b) “T” transverse direction parallel to direction of shearing 20 25 Shear disp 2 mm Shear disp 3 mm 16 Shear force (N Shear force (N 20 Shear disp 2 mm Shear disp 3 mm 15 10 12 8 4 5 0 0 0 1 2 Displacement (mm) 0 3 1 (a) 2 Displacement (mm) 3 (b) Figure 15. Measured force-displacement relationships, after correction for friction eﬀects: (a) “M” machine direction parallel to direction of shearing; (b) “T” transverse direction parallel to direction of shearing 18 of 23 American Institute of Aeronautics and Astronautics see Table 4. With everything else ﬁxed, one ﬁnds that the greater the shear displacement, the greater the shear force is. Also, for the same displacement, the ﬁlm arranged with the machine direction parallel to the long edge carries a higher shear force than the ﬁlm placed in the transverse direction; however the diﬀerence is generally less than 10%. This is because Stratoﬁlm 420 has only a weak anisotropy. Table 4. Maximum shear forces Test No. Direction of ﬁlm Displacement δx (mm) Max total horizontal force F (N) Max shear force S (N) VII. a M 2.31 17.618 16.320 b M 3.36 21.206 19.908 c T 2.39 16.633 15.335 d T 3.34 19.271 17.973 Comparison of Results and Discussion Displacement δ Displacement δ The general orthotropic viscoelastic membrane model can be tested by comparing the simulation results to the results from the experiments. The ﬁrst issue is how many steps should be used to represent the time history of the imposed displacement. As an example, we have investigated the linear loading ramp for the M test with a displacement δx = 3.36 mm, at the time tL = 10.775 s. We have found that the total estimate for the shear force at this time increases from 16.445 N, to 18.970 N and 20.117 N for single-step, two-step and three-step approximations, respectively The ﬁrst two results diﬀer by 15% but the diﬀerence of the last two reduces to 6%. Taking 20.117 N as the correct solution, we have assumed that a two-step approximation for linear ramp loading is suﬃciently accurate. The experimental measurement of the force at this time was 19.908 N, which conﬁrm that the two-step solution is close to the physically correct value. Based on this observation, Figure 16 shows the discretization technique that has been adopted for the actual displacement function, depending on where the chosen time t falls with respect to the ramp times. 0 t tL 0 tL Time (a) t tL+ tC Displacement δ Time (b) 0 tL tL+ tC t Time (c) Figure 16. Discretization of displacement function using two-steps for each ramp; (a) case t < tL ; (b) case tL < t < tL + tC ; (c) case tL + tC < t < tL + tC + tU . 19 of 23 American Institute of Aeronautics and Astronautics The ﬁrst thing to note from the simulation results is that the wrinkling angles are on average 44.6◦ and 48.3◦ , respectively, in the M and T cases. This diﬀerenc eis too small to be detected in the experiments. Figures 17 and 18 compare the relationships between total shear force and time obtained from the simulations with both uncorrected and friction corrected experimental results. During the initial loading, especially the ﬁrst 1 s, the comparison shows signiﬁcant diﬀerences however this is not surprising. The diﬀerences are due to the presence of inertia forces in the experimental results, due to the mass of the edge block that was not included in the ﬁnite-element model, and to the fact that when the shear forces are small the force sensor is less accurate and also friction is comparatively large and so our rather rough technique for removing friction eﬀects is not accurate. The simulations and the experimental results are much closer from t ≈ 2 s onwards and particularly for the case δx = 3 mm. In Figure 17(b) during the constant displacement phase the maximum diﬀerence between simulation and friction-corrected measured shear forces is 0.83 N, or 7.15%. In Figure 18(b1), the maximum diﬀerence the maximum diﬀerence is 0.58 N, or 5.28%. Figure 18(b2) shows a detail of the unloading part of the plot shown in Figure 18(b1), to provide a more detailed comparison of the unloading curves. In this range the maximum diﬀerence is 0.74 N. 10 2 10 2 Total horizontal force Shear force Simulation 10 1 10 0 Force (N) Force (N) Total horizontal force Shear force Simulation −1 10 0 10 1 10 2 10 Time (s) 3 10 4 10 10 1 10 0 −1 10 5 10 0 10 1 10 2 10 Time (s) 3 10 4 10 5 10 (b) (a) Figure 17. Comparison between simulation and measurement for “M” test: (a) maximum shear displacement 2 mm; (b) maximum shear displacement 3 mm Figure 19 shows the hysteretic relationship between shear force and displacement. Diﬀerent loading and unloading paths result from the cumulative eﬀects of viscoelasticity, which has a signiﬁcant inﬂuence on the behavior of the wrinkled ﬁlms. VIII. Conclusion The objective of this study was to investigate the wrinkling of orthotropic viscoelastic membranes. The method developed in this paper, based on a modiﬁcation of the material stiﬀness matrix to incorporate the eﬀects of orthotropic wrinkling and viscoelasticity, has been shown to be an eﬀective way of capturing in a ﬁnite element simulation the behavior of a real plastic ﬁlm. In the wrinkling model the state of a membrane element (taut, wrinkled, slack) is deﬁned by a mixed criterion. Once it has been established that an element is wrinkled, an iterative scheme searches for the wrinkle orientation angle and the correct stress distribution, involving only uniaxial tension in the wrinkle direction, is then obtained. This wrinkling model has been validated by a comparison with a published solution for the case of a timeindependent isotropic membrane under simple shear. The model has then been applied to a particular type of viscoelastic balloon ﬁlm, known as StratoFilm 420. Using the Rand-Schapery model for this ﬁlm, a timedependent pseudo-elastic stiﬀness matrix was deﬁned and so, instead of having to compute the convolution integral throughout the simulation, we were able to compute the behavior of a membrane structure by superposition of a series of incremental response functions. These calculations were implemented in standard 20 of 23 American Institute of Aeronautics and Astronautics 10 2 14 Total horizontal force Shear force Simulation 12 10 Force (N Force (N) 10 1 10 8 6 0 Total horizontal force Shear force Simulation 10 -1 10 −1 4 2 0 10 0 10 1 10 2 Time (s) 10 3 10 4 0 10 5 1 2 3 2 7 8 +22,125.67 s 14 12 Total horizontal force Shear force Simulation 10 Force (N) 10 1 Force (N) 6 (a2) (a1) 10 4 5 Time (s) Total horizontal force Shear force Simulation 10 0 8 6 4 2 10 −1 10 −1 0 10 0 10 1 10 2 10 3 10 4 10 5 0 1 2 Time (s) (b1) 3 4 5 Time (s) 6 7 8 +21,978.79 s (b2) Figure 18. Comparison between simulation and experiment for “T” test: (a1) full behavior for maximum shear displacement 2 mm; (a2) unloading curve for maximum shear displacement 2 mm; (b1) full behavior for maximum shear displacement 3 mm; (b2) unloading curve for maximum shear displacement 3 mm 21 of 23 American Institute of Aeronautics and Astronautics 20 Total horizontal force Shear force Simulation 16 Total horizontal force Shear force Simulation 16 Force (N Force (N 12 8 4 12 8 4 0 0 1 Displacement (mm) 0 2 0 1 (a) 2 Displacement (mm) 3 (b) Figure 19. Comparison between simulation and experiment for “T” test: (a) maximum shear displacement 2 mm; (b) maximum shear displacement 3 mm ﬁnite element software. Experimental tests on StratoFilm 420 under simple shear were carried out, including loading and unloading, and the experimental results were compared with ABAQUS/Explicit simulations. The results agree very well once friction and dynamic eﬀects are excluded. There are diﬀerences of about 10% in the shear forces measured on membranes arranged in diﬀerent material directions, as StratoFilm 420 has only weak anisotropy and so the direction of the wrinkles changed by less than 4◦ when the ﬁlm was rotated through 90◦ . Signiﬁcant diﬀerences were seen between loading and unloading curves, indicating that viscoelastic behavior is a signiﬁcant source of energy dissipation. Acknowledgments We thank the NASA Super-Pressure Balloon team for their contributions to this research. In particular, Dr Loren Seely (Aerostar International) has provided ﬁlm samples, Dr David Wakeﬁeld (Tensys Dynamics Ltd) and Dr Jim Rand (Winzen Engineering, Inc.) have helped with many comments. This research was supported by the NASA Balloon Program Oﬃce (contract monitor Danny Ball). References 1 Deng, X. and S. Pellegrino, Computation of partially inflated shapes of stratospheric balloon structures, 48th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, 7-10 April 2008, Schaumburg, Illinois, AIAA-2008-2133. 2 Deng, X. and Pellegrino, S., “Finite element simulations of clefting in lobed super-pressure balloons,” AIAA Balloon Systems Conference, 4-7 May 2009, Seattle, Washington, AIAA-2009-2816. 3 Ward, I.M., Mechanical Properties of Solid Polymers, 2nd edition, John Wiley & Sons, 1985. 4 McCrum, N.G., Buckley, C.P., and Bucknall, C.B. Principles of Polymer Engineering, 2nd edition, Oxford Science Publications, Oxford, 2003. 5 Schapery, R. A., “On the Characterization of Nonlinear Viscoelastic Material,” Polymer Engineering and Science, Vol. 9, No. 4, July, 1969, pp. 295–310. 6 Schapery, R. A., “Nonlinear Viscoelastic and Viscoelastic Constitutive Equations Based on Thermodynamics,” Mechanics of Time-Dependent Material, Vol. 1, Dec. 1997, pp. 209–240. 7 Wong, Y.W., and Pellegrino, S., Wrinkled membranes. Part I: experiments. Journal of Mechanics of Materials and Structures, Vol. 1, 1-23, 2006. 8 Wong, Y.W., and Pellegrino, S., Wrinkled membranes. Part II: analytical models. Journal of Mechanics of Materials and Structures, Vol. 1, 25-59, 2006. 9 Wong, Y.W., and Pellegrino, S., Wrinkled membranes. Part III: numerical simulations. Journal of Mechanics of Materials and Structures, Vol. 1, 61-93, 2006. 22 of 23 American Institute of Aeronautics and Astronautics 10 Kang, S. and Im, S., “Finite Element Analysis of Wrinkling Membranes,” Journal of Applied Mechanics, Vol. 64, Jun. 1997, pp. 263–269. 11 Gerngross, T., and Pellegrino, S., Implementation and validation of Schapery-Rand anisotropic viscoelasticity model for super-pressure balloons. AIAA Balloon Systems Conference, 21-24 May, 2007, Williamsburg, VA, 2007. 12 Gerngross, T., and Pellegrino, S., Modelling of anisotropic viscoelastic behaviour in super-pressure balloons. 48th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, 23-26 April 2007, Honolulu, Hawaii, 2007. 13 Gerngross, T., and Pellegrino, S., Anisotropic viscoelasticity and wrinkling of superpressure balloons: simulation and experimental verification. AIAA Balloon Systems Conference, 4-7 May 2009, Seattle, WA, 2009. 14 Epstein, M., and Forcinito, M.A., Anisotropic membrane wrinkling: theory and analysis. International Journal of Solids and Structures, Vol. 38, 5253-5272, 2001. 15 Raible, T., Tegeler, K., Lohnert, S., and Wriggers, P., Development of a wrinkling algorithm for orthotropic membrane materials. Computer Methods in Applied Mechanics and Engineering, Vol. 194, 2550-2568, 2005. 16 Rand, J.L., “An Improved Constitutive Equation for SF420, Part I: the Master Curve,” Internal Report, Winzen Engineering Inc, July. 2008. 17 Rand, J. L., “An Improved Constitutive Equation for SF420, Part II: the Biaxial Behavior,” Internal Report, Winzen Engineering Inc, July. 2008. 18 Rainwater, E.L., and Smith, M.S., Ultra high altitude balloons for medium-to-large payloads, Advances in Space Research, Volume 33, Issue 10, 2004, 1648-1652. 23 of 23 American Institute of Aeronautics and Astronautics